Binary Mixture Composed of Nematic Liquid Crystal and Carbon Nanotubes: A Theoretical Description

Vlad Popa-Nita and Robert Repnik

## Abstract

Based on the phenomenological model first presented by van der Schoot et al., which predicts the alignment of carbon nanotube (CNT) dispersions in thermotropic nematic liquid crystals, we present the extensive results concerning the phase diagram and the orientational properties of the mixture in this chapter.

Keywords: liquid crystal, carbon nanotube, phase transition

## 1. Introduction

A method to obtain aligned CNTs (necessary for applications) is to disperse them into liquid crystals (LCs) [with their self-organization (long-range orientational order) and fluidity] [1–9]. The thermotropic [10–13] and the lyotropic LCs [14–17] have been used to align CNTs parallel as well as perpendicular to average direction of alignment of long axes of LC molecules called the director. As a consequence, the orientational order parameter of CNTs could have the values between 0:6 and 0:9. The study of mixture composed by LCs and CNTs is also important due to the influence of CNTs on the physical properties of LCs (increased dielectric anisotropy, decreased threshold voltage, much accelerated electrooptical response) [18–25].

The main hypothesis used in the theoretical study of the collective behavior of CNTs dispersed in the isotropic solvents [26–28] as well as in LCs [29–36] is that they can be considered as rigid rod polymers [37].

Using the density functional theory, the isotropic-liquid crystal phase transition has been analyzed considering the van der Waals attractive interactions [26]. Onsager theory of rigid rods [38] was used to study the phase behavior of CNTs dispersed into organic and aqueous solutions [27]. Also, the Onsager model including length polydispersity and solvent-mediated interaction was considered to study the dispersions of CNTs in superacids [28]. These theoretical studies lead to the conclusion that to obtain orientational order of CNTs at room temperature it is necessary that the van der Waals interactions must be screened out, i.e., the CNTs must be dispersed in a good solvent. In the case of a non-good solvent, no liquid crystalline phases of CNTs form at room temperature because only dilute solutions are thermodynamically stable.

Matsuyama [29, 30] used a mean field theory to analyze the phase behavior of a mixture composed of low-molecular-weight liquid crystal and a rigid rod-like polymer such as CNTs. The free energy is constructed on the basis of Onsager model for excluded volume interactions, the Maier-Saupe model for orientational-dependent attractive interactions, and the Flory-Huggins theory for binary mixtures.

above are those used in this paper. In Eq. (2), kB is the Boltzmann constant, T is the absolute temperature, ϕ represents the volume fraction of CNTs, 1 � ϕ defines the

Binary Mixture Composed of Nematic Liquid Crystal and Carbon Nanotubes: A Theoretical…

Eq. (2) defines a first-order isotropic-nematic phase transition of CNTs with the equilibrium values of the order parameters SCNT,iso ¼ 0 and SCNT,nem ¼ 0:3365 and of the volume fractions, respectively, ϕiso ¼ 0:01349 and ϕnem ¼ 0:01351. These equilibrium values of the parameters are obtained minimizing the free energy (2) with respect to SCNT and equating the chemical potentials of CNTs (μCNT ¼ vCNT <sup>f</sup> CNT <sup>þ</sup> ð Þ <sup>1</sup> � <sup>ϕ</sup> <sup>∂</sup><sup>f</sup> CNT=∂<sup>ϕ</sup> ) and of LC (μLC <sup>¼</sup> vLC <sup>f</sup> CNT � <sup>ϕ</sup>∂<sup>f</sup> CNT=∂<sup>ϕ</sup> <sup>Þ</sup> in the two phases. The model predicts a relative variation of the volume fraction of CNTs (the Flory "chimney") at the transition of 0.19%, while the prediction of Onsager and Flory [38, 46] for monodisperse lyotropic LC is about 1%, and the experimental results obtained by the polarized light microscopy for an aqueous dispersion of multiwall carbon nanotube indicate a biphasic region that range between 1 and 4% [47, 48]. The discrepancy is due to polydispersity, as well as the possibility of

To characterize the isotropic-nematic phase transition of thermotropic LC, we

where T<sup>∗</sup> is the undercooling limit temperature of stability of the isotropic phase

The condition of weak anchoring limit of the interaction between the two components is <sup>D</sup> <sup>≪</sup> <sup>ξ</sup>, where the diameter of a CNT is <sup>D</sup> <sup>≈</sup>2 nm and <sup>ξ</sup> <sup>¼</sup> <sup>K</sup>=<sup>W</sup> <sup>≈</sup> <sup>10</sup>�<sup>5</sup> <sup>m</sup> is

The coupling free energy has been explained in [31], and it has the following form:

the elastic penetration length (K ≈10�<sup>11</sup> N is a typical elastic constant, and

<sup>f</sup> CNT=LC ¼ �γϕSLCSCNT <sup>1</sup> � <sup>1</sup>

energy, the coupling parameter in the case of thin rods is larger than that of the thick one. From the experimental results, we find that the value of the coupling parameter can be between 10�<sup>3</sup> � <sup>10</sup><sup>3</sup> <sup>N</sup> � <sup>m</sup>�2. In the limit of large coupling

We note that positive values of γ characterize a parallel alignment of LC molecules to CNTs. In this chapter we extend our analysis considering also negative

γ ! ∞, the orientational order of CNTs is perfect SCNT ! 1.

LC � <sup>3</sup> 4 BS<sup>3</sup> LC þ 9 4 CS<sup>4</sup>

LC (3)

, <sup>B</sup>≈7:<sup>1</sup> � <sup>10</sup><sup>5</sup> <sup>J</sup> � <sup>m</sup>�3, and

=24aC ¼ 308:95 K with SLC,iso ¼ 0 and

2

<sup>3</sup> W=D defines the coupling parameter. Thus, for the same anchoring

SCNT (4)

a T � <sup>T</sup><sup>∗</sup> ð ÞS<sup>2</sup>

and the constant coefficients a, B, and C depend on the material. Later, in our numerical calculations presented in Section 3, we consider the following values:

<sup>C</sup>≈4:<sup>3</sup> � 105 <sup>J</sup> � <sup>m</sup>�<sup>3</sup> [40, 49–51], values specific for pentylcyanobiphenyl (5CB). For this nematogen, the first-order isotropic-nematic phase transition takes place at

volume fraction of the LC, and L ¼ L0=D is the aspect ratio of a CNT.

segregation which the model does not consider.

DOI: http://dx.doi.org/10.5772/intechopen.81936

2.2 Free energy of thermotropic liquid crystal

<sup>f</sup> LC <sup>¼</sup> ð Þ <sup>1</sup> � <sup>ϕ</sup> <sup>3</sup>

2

use the Landau-de Gennes [39] free energy:

<sup>T</sup><sup>∗</sup> <sup>¼</sup> <sup>307</sup>:55 K, <sup>a</sup>≈3:<sup>5</sup> � <sup>10</sup><sup>4</sup> <sup>J</sup> � <sup>m</sup>�<sup>3</sup> � <sup>K</sup>�<sup>1</sup>

W ≈ 10�<sup>6</sup> N=m is a typical anchoring energy).

temperature <sup>T</sup> <sup>¼</sup> TNI <sup>¼</sup> <sup>T</sup><sup>∗</sup> <sup>þ</sup> <sup>B</sup><sup>2</sup>

2.3 The coupling free energy

SLC,nem ¼ B=6C ¼ 0:2752.

where <sup>γ</sup> � <sup>4</sup>

35

In the previous papers [31, 32, 34–36], we have presented a phenomenological theory to describe the alignment of CNT dispersions in thermotropic nematic LCs. We combined the Landau-de Gennes [39, 40] free energy for thermotropic ordering of the LC solvent and the Doi free energy [41–43] for the lyotropic orientational order of CNTs. Because the CNT is much thinner than the elastic penetration length, the alignment of CNTs in the nematic solvent is caused by the coupling of the LC director field to the anisotropic interfacial tension of the CNTs. This is true only for very dilute solutions without large aggregates [33]. Density functional calculations [44] show that CNT alignment mechanism in LC is associated with a strong interaction due to surface anchoring with a binding energy of �2eV for π � π electron stacking between LC molecules and CNT.

In the present chapter, we extend this model to generalize the anisotropic interaction form between a CNT and the liquid crystal molecules including the possibility of perpendicular alignment.

The remainder of this chapter is organized as follows. In Section 2, we describe the model. In Section 3, we illustrate the results and finally give the main conclusions in Section 4.

## 2. Model

The free energy density of the binary mixture composed of CNTs and thermotropic nematic LC contains three terms:

$$f = f\_{\rm CNT} + f\_{\rm LC} + f\_{\rm CNT/LC} \tag{1}$$

where f CNT represents the Doi free energy density of CNTs, f LC represents the Landau-de Gennes free energy density of the nematic liquid crystal order, and f CNT=LC takes into account the interaction of these two components.

#### 2.1 Free energy of carbon nanotubes

At the mesoscopic level of description, the free energy of CNTs can be written in the following form [31]:

$$\begin{aligned} f\_{\text{CNT}} &= k\_B T \left[ \frac{\mathbf{1}}{\upsilon\_{\text{LC}}} (\mathbf{1} - \boldsymbol{\phi}) \ln \left( \mathbf{1} - \boldsymbol{\phi} \right) + \frac{\mathbf{1}}{\upsilon\_{\text{CNT}}} \boldsymbol{\phi} \ln \boldsymbol{\phi} \right] \\ &+ k\_B T \frac{L \boldsymbol{\phi}^2}{\mathsf{\dot{\sigma} \upsilon\_{\text{CNT}}}} \left[ \left( \frac{\mathbf{3}}{L \boldsymbol{\phi}} - \mathbf{1} \right) \mathbf{S}\_{\text{CNT}}^2 - \frac{2}{3} \mathbf{S}\_{\text{CNT}}^3 + \mathbf{S}\_{\text{CNT}}^4 \right] \end{aligned} \tag{2}$$

where the first two terms represent the entropy of isotropic mixing of CNTs and LC components [45] and the third one is obtained from the Onsager theory [38] using the Smoluchowski Equation [41, 42]. In this form, the van der Waals attractions between CNTs are neglected. The long-ranged intermolecular attractions between CNTs were considered in [36]. vLC ≈πld<sup>2</sup> =4 represents the volume of one LC molecule with length l ≈3 nm and diameter d≈ 0:5 nm, and vCNT ≈πL0D<sup>2</sup> =4 is the volume of one CNT with length L<sup>0</sup> ≈400 nm and diameter D ≈ 2 nm. The values cited

Binary Mixture Composed of Nematic Liquid Crystal and Carbon Nanotubes: A Theoretical… DOI: http://dx.doi.org/10.5772/intechopen.81936

above are those used in this paper. In Eq. (2), kB is the Boltzmann constant, T is the absolute temperature, ϕ represents the volume fraction of CNTs, 1 � ϕ defines the volume fraction of the LC, and L ¼ L0=D is the aspect ratio of a CNT.

Eq. (2) defines a first-order isotropic-nematic phase transition of CNTs with the equilibrium values of the order parameters SCNT,iso ¼ 0 and SCNT,nem ¼ 0:3365 and of the volume fractions, respectively, ϕiso ¼ 0:01349 and ϕnem ¼ 0:01351. These equilibrium values of the parameters are obtained minimizing the free energy (2) with respect to SCNT and equating the chemical potentials of CNTs (μCNT ¼ vCNT <sup>f</sup> CNT <sup>þ</sup> ð Þ <sup>1</sup> � <sup>ϕ</sup> <sup>∂</sup><sup>f</sup> CNT=∂<sup>ϕ</sup> ) and of LC (μLC <sup>¼</sup> vLC <sup>f</sup> CNT � <sup>ϕ</sup>∂<sup>f</sup> CNT=∂<sup>ϕ</sup> <sup>Þ</sup> in the two phases. The model predicts a relative variation of the volume fraction of CNTs (the Flory "chimney") at the transition of 0.19%, while the prediction of Onsager and Flory [38, 46] for monodisperse lyotropic LC is about 1%, and the experimental results obtained by the polarized light microscopy for an aqueous dispersion of multiwall carbon nanotube indicate a biphasic region that range between 1 and 4% [47, 48]. The discrepancy is due to polydispersity, as well as the possibility of segregation which the model does not consider.

#### 2.2 Free energy of thermotropic liquid crystal

To characterize the isotropic-nematic phase transition of thermotropic LC, we use the Landau-de Gennes [39] free energy:

$$f\_{LC} = (1 - \phi) \left[ \frac{3}{2} a (T - T^\*) S\_{LC}^2 - \frac{3}{4} B S\_{LC}^3 + \frac{9}{4} C S\_{LC}^4 \right] \tag{3}$$

where T<sup>∗</sup> is the undercooling limit temperature of stability of the isotropic phase and the constant coefficients a, B, and C depend on the material. Later, in our numerical calculations presented in Section 3, we consider the following values: <sup>T</sup><sup>∗</sup> <sup>¼</sup> <sup>307</sup>:55 K, <sup>a</sup>≈3:<sup>5</sup> � <sup>10</sup><sup>4</sup> <sup>J</sup> � <sup>m</sup>�<sup>3</sup> � <sup>K</sup>�<sup>1</sup> , <sup>B</sup>≈7:<sup>1</sup> � <sup>10</sup><sup>5</sup> <sup>J</sup> � <sup>m</sup>�3, and <sup>C</sup>≈4:<sup>3</sup> � 105 <sup>J</sup> � <sup>m</sup>�<sup>3</sup> [40, 49–51], values specific for pentylcyanobiphenyl (5CB). For this nematogen, the first-order isotropic-nematic phase transition takes place at temperature <sup>T</sup> <sup>¼</sup> TNI <sup>¼</sup> <sup>T</sup><sup>∗</sup> <sup>þ</sup> <sup>B</sup><sup>2</sup> =24aC ¼ 308:95 K with SLC,iso ¼ 0 and SLC,nem ¼ B=6C ¼ 0:2752.

#### 2.3 The coupling free energy

The condition of weak anchoring limit of the interaction between the two components is <sup>D</sup> <sup>≪</sup> <sup>ξ</sup>, where the diameter of a CNT is <sup>D</sup> <sup>≈</sup>2 nm and <sup>ξ</sup> <sup>¼</sup> <sup>K</sup>=<sup>W</sup> <sup>≈</sup> <sup>10</sup>�<sup>5</sup> <sup>m</sup> is the elastic penetration length (K ≈10�<sup>11</sup> N is a typical elastic constant, and W ≈ 10�<sup>6</sup> N=m is a typical anchoring energy).

The coupling free energy has been explained in [31], and it has the following form:

$$\int f\_{\rm{CNT/LC}} = -\chi \phi \mathbf{S}\_{\rm{LC}} \mathbf{S}\_{\rm{CNT}} \left( \mathbf{1} - \frac{\mathbf{1}}{2} \mathbf{S}\_{\rm{CNT}} \right) \tag{4}$$

where <sup>γ</sup> � <sup>4</sup> <sup>3</sup> W=D defines the coupling parameter. Thus, for the same anchoring energy, the coupling parameter in the case of thin rods is larger than that of the thick one. From the experimental results, we find that the value of the coupling parameter can be between 10�<sup>3</sup> � <sup>10</sup><sup>3</sup> <sup>N</sup> � <sup>m</sup>�2. In the limit of large coupling γ ! ∞, the orientational order of CNTs is perfect SCNT ! 1.

We note that positive values of γ characterize a parallel alignment of LC molecules to CNTs. In this chapter we extend our analysis considering also negative

Matsuyama [29, 30] used a mean field theory to analyze the phase behavior of a mixture composed of low-molecular-weight liquid crystal and a rigid rod-like polymer such as CNTs. The free energy is constructed on the basis of Onsager model for excluded volume interactions, the Maier-Saupe model for orientational-dependent

In the previous papers [31, 32, 34–36], we have presented a phenomenological theory to describe the alignment of CNT dispersions in thermotropic nematic LCs. We combined the Landau-de Gennes [39, 40] free energy for thermotropic ordering of the LC solvent and the Doi free energy [41–43] for the lyotropic orientational order of CNTs. Because the CNT is much thinner than the elastic penetration length, the alignment of CNTs in the nematic solvent is caused by the coupling of the LC director field to the anisotropic interfacial tension of the CNTs. This is true only for very dilute solutions without large aggregates [33]. Density functional calculations [44] show that CNT alignment mechanism in LC is associated with a strong interaction due to surface anchoring with a binding energy of �2eV for π � π

In the present chapter, we extend this model to generalize the anisotropic interaction form between a CNT and the liquid crystal molecules including the possibil-

The remainder of this chapter is organized as follows. In Section 2, we describe the model. In Section 3, we illustrate the results and finally give the main conclu-

The free energy density of the binary mixture composed of CNTs and thermo-

where f CNT represents the Doi free energy density of CNTs, f LC represents the Landau-de Gennes free energy density of the nematic liquid crystal order, and

At the mesoscopic level of description, the free energy of CNTs can be written in

ð Þ <sup>1</sup> � <sup>ϕ</sup> ln 1ð Þþ � <sup>ϕ</sup> <sup>1</sup>

where the first two terms represent the entropy of isotropic mixing of CNTs and LC components [45] and the third one is obtained from the Onsager theory [38] using the Smoluchowski Equation [41, 42]. In this form, the van der Waals attractions between CNTs are neglected. The long-ranged intermolecular attractions between

ume of one CNT with length L<sup>0</sup> ≈400 nm and diameter D ≈ 2 nm. The values cited

3 <sup>L</sup><sup>ϕ</sup> � <sup>1</sup> 

S2 CNT � <sup>2</sup> 3 S3 CNT <sup>þ</sup> <sup>S</sup><sup>4</sup>

f CNT=LC takes into account the interaction of these two components.

cule with length l ≈3 nm and diameter d≈ 0:5 nm, and vCNT ≈πL0D<sup>2</sup>

f ¼ f CNT þ f LC þ f CNT=LC (1)

vCNT

ϕln ϕ

(2)

=4 represents the volume of one LC mole-

CNT

=4 is the vol-

attractive interactions, and the Flory-Huggins theory for binary mixtures.

Liquid Crystals - Self-Organized Soft Functional Materials for Advanced Applications

electron stacking between LC molecules and CNT.

ity of perpendicular alignment.

tropic nematic LC contains three terms:

2.1 Free energy of carbon nanotubes

<sup>f</sup> CNT <sup>¼</sup> kBT <sup>1</sup>

CNTs were considered in [36]. vLC ≈πld<sup>2</sup>

vLC

<sup>þ</sup> kBT <sup>L</sup>ϕ<sup>2</sup> 6vCNT

the following form [31]:

34

sions in Section 4.

2. Model

values of γ which characterize a perpendicular alignment. Depending on the orientational order parameters SCNT and SLC, two nematic phases could be defined: (i) the N<sup>1</sup> phase with SCNT > 0 and SLC > 0 (parallel alignment of CNT and LC molecules) and (ii) the N<sup>2</sup> phase with SCNT < 0 and SLC > 0 (perpendicular alignment of CNT and LC molecules). These two phases are experimentally obtained depending on the surface treatment of the CNTs.

### 2.4 The total free energy density of the binary mixture

Finally, the total free energy density of the binary mixture (1) is the sum of the free energy densities of CNTs (2), thermotropic LC (3), and interaction between nematic CNTs and nematic LC (4):

$$\begin{aligned} f &= k\_B T \left[ \frac{1}{\nu\_{LC}} \left( 1 - \phi \right) \ln \left( 1 - \phi \right) + \frac{1}{\nu\_{CNT}} \phi \ln \phi \right] \\ &+ k\_B T \frac{L \phi^2}{6 \nu\_{CNT}} \left[ \left( \frac{3}{L \phi} - 1 \right) S\_{CNT}^2 - \frac{2}{3} S\_{CNT}^3 + S\_{CNT}^4 \right] \\ &+ (1 - \phi) \left[ \frac{3}{2} a (T - T^\*) S\_{LC}^2 - \frac{3}{4} B S\_{LC}^3 + \frac{9}{4} C S\_{LC}^4 \right] \\ &- \gamma \phi S\_{LC} S\_{CNT} \left( 1 - \frac{1}{2} S\_{CNT} \right) \end{aligned} \tag{5}$$

The dependence of γ<sup>c</sup> on the lengths of CNTs for a fixed value of the temperature is shown in Figure 2 (we mention that for the value of the temperature shown (T � TNI ¼ �1:4K) the LC is in the nematic phase). The critical value of the coupling parameter decreases when the length of CNTs increase, meaning that the

Binary Mixture Composed of Nematic Liquid Crystal and Carbon Nanotubes: A Theoretical…

In Figure 3 the volume fractions of CNTs at the transition as a function of the coupling parameter for a fixed value of the temperature are shown. For negative values of γ (region I in the figure, perpendicular alignment), the volume fraction

The critical value of the coupling parameter γ<sup>c</sup> as a function of the lengths of CNTs for a fixed temperature in

The volume fractions of CNTs at the transition as a function of coupling parameter for a fixed value of

continuous paranematic-nematic transition of CNTs is favored.

The critical value of the coupling parameter γ<sup>c</sup> as a function of temperature.

DOI: http://dx.doi.org/10.5772/intechopen.81936

Figure 1.

Figure 2.

Figure 3.

37

the nematic region of the liquid crystal.

temperature in the nematic region of LC.

## 3. Results

We present the main results concerning the phase behavior of the CNT-LC binary mixture as a function of temperature, volume fraction ϕ of CNTs, and coupling strength γ.

### 3.1 Positive γ: critical point of CNT phase transition

The positive value of the interaction parameter γ defines the nematic N<sup>1</sup> phase with SCNT > 0 and SLC > 0 (the rod and the LC molecules are parallel to each other). The isotropic phase of CNTs is transformed into a nematic phase with a small degree of order which is called paranematic phase (by analogy with the magnetism). The phase transition nematic-paranematic of the CNTs is first order for small values of the interaction parameter (so-called subcritical regime of CNTs). For large values of γ, the phase transition of CNTs becomes continuous. The critical point is given by the equations <sup>∂</sup><sup>f</sup> <sup>=</sup>∂SCNT <sup>¼</sup> <sup>∂</sup><sup>2</sup> f =∂S<sup>2</sup> CNT <sup>¼</sup> <sup>∂</sup><sup>3</sup><sup>f</sup> <sup>=</sup>∂S<sup>3</sup> CNT ¼ 0, giving SCNT,c ¼ 1=6 and the effective volume fraction ð Þ Lϕ <sup>c</sup> ¼ 2:592, while the critical value of the interaction parameter is given by the equation:

$$\gamma\_c = \frac{k\_B T}{125 \nu\_{\rm CNT} \mathbb{S}\_{LC,c}}.\tag{6}$$

The dependence of γ<sup>c</sup> as a function of temperature is shown in Figure 1.

In the nematic phase of the liquid crystal, the critical interaction parameter is relatively small (because SLC,c has relatively large values between 0.28 and 0.8), while in the isotropic phase of the liquid crystal, the value of the order parameter is very small (≃10�4), and the values of γ<sup>c</sup> are relatively large. As a consequence there is a jump of γ<sup>c</sup> at TNI.

Binary Mixture Composed of Nematic Liquid Crystal and Carbon Nanotubes: A Theoretical… DOI: http://dx.doi.org/10.5772/intechopen.81936

Figure 1.

values of γ which characterize a perpendicular alignment. Depending on the orientational order parameters SCNT and SLC, two nematic phases could be defined: (i) the N<sup>1</sup> phase with SCNT > 0 and SLC > 0 (parallel alignment of CNT and LC molecules) and (ii) the N<sup>2</sup> phase with SCNT < 0 and SLC > 0 (perpendicular alignment of CNT and LC molecules). These two phases are experimentally obtained

Liquid Crystals - Self-Organized Soft Functional Materials for Advanced Applications

Finally, the total free energy density of the binary mixture (1) is the sum of the free energy densities of CNTs (2), thermotropic LC (3), and interaction between

vCNT

ϕln ϕ

CNT

CNT ¼ 0, giving SCNT,c ¼ 1=6

: (6)

(5)

ð Þ <sup>1</sup> � <sup>ϕ</sup> ln 1ð Þþ � <sup>ϕ</sup> <sup>1</sup>

3 <sup>L</sup><sup>ϕ</sup> � <sup>1</sup> 

a T � <sup>T</sup><sup>∗</sup> ð ÞS<sup>2</sup>

2 SCNT 

We present the main results concerning the phase behavior of the CNT-LC binary mixture as a function of temperature, volume fraction ϕ of CNTs, and

The positive value of the interaction parameter γ defines the nematic N<sup>1</sup> phase with SCNT > 0 and SLC > 0 (the rod and the LC molecules are parallel to each other). The isotropic phase of CNTs is transformed into a nematic phase with a small degree of order which is called paranematic phase (by analogy with the magnetism). The phase transition nematic-paranematic of the CNTs is first order for small values of the interaction parameter (so-called subcritical regime of CNTs). For large values of γ, the phase transition of CNTs becomes continuous. The critical point is

f =∂S<sup>2</sup>

and the effective volume fraction ð Þ Lϕ <sup>c</sup> ¼ 2:592, while the critical value of the

<sup>γ</sup><sup>c</sup> <sup>¼</sup> kBT

The dependence of γ<sup>c</sup> as a function of temperature is shown in Figure 1. In the nematic phase of the liquid crystal, the critical interaction parameter is relatively small (because SLC,c has relatively large values between 0.28 and 0.8), while in the isotropic phase of the liquid crystal, the value of the order parameter is very small (≃10�4), and the values of γ<sup>c</sup> are relatively large. As a consequence there

125vCNTSLC,c

CNT <sup>¼</sup> <sup>∂</sup><sup>3</sup><sup>f</sup> <sup>=</sup>∂S<sup>3</sup>

S2 CNT � <sup>2</sup> 3 S3 CNT <sup>þ</sup> <sup>S</sup><sup>4</sup>

LC � <sup>3</sup> 4 BS<sup>3</sup> LC þ 9 4 CS<sup>4</sup> LC

depending on the surface treatment of the CNTs.

nematic CNTs and nematic LC (4):

3. Results

coupling strength γ.

is a jump of γ<sup>c</sup> at TNI.

36

<sup>f</sup> <sup>¼</sup> kBT <sup>1</sup>

vLC

<sup>þ</sup> kBT <sup>L</sup>ϕ<sup>2</sup> 6vCNT

<sup>þ</sup> ð Þ <sup>1</sup> � <sup>ϕ</sup> <sup>3</sup>

2

� γϕSLCSCNT <sup>1</sup> � <sup>1</sup>

3.1 Positive γ: critical point of CNT phase transition

given by the equations <sup>∂</sup><sup>f</sup> <sup>=</sup>∂SCNT <sup>¼</sup> <sup>∂</sup><sup>2</sup>

interaction parameter is given by the equation:

2.4 The total free energy density of the binary mixture

The critical value of the coupling parameter γ<sup>c</sup> as a function of temperature.

The dependence of γ<sup>c</sup> on the lengths of CNTs for a fixed value of the temperature is shown in Figure 2 (we mention that for the value of the temperature shown (T � TNI ¼ �1:4K) the LC is in the nematic phase). The critical value of the coupling parameter decreases when the length of CNTs increase, meaning that the continuous paranematic-nematic transition of CNTs is favored.

In Figure 3 the volume fractions of CNTs at the transition as a function of the coupling parameter for a fixed value of the temperature are shown. For negative values of γ (region I in the figure, perpendicular alignment), the volume fraction

#### Figure 2.

The critical value of the coupling parameter γ<sup>c</sup> as a function of the lengths of CNTs for a fixed temperature in the nematic region of the liquid crystal.

#### Figure 3.

The volume fractions of CNTs at the transition as a function of coupling parameter for a fixed value of temperature in the nematic region of LC.

Figure 4.

The order parameter of the two phases of CNTs at the transition as a function of the coupling parameter for a fixed value of the temperature in the nematic region of LC.

gap of CNTs remains practically constant, while for positive values (region II in the figure, parallel alignment), the volume fraction gap decreases with increasing γ until it cancels for critical value γc.

The CNT order parameters at the transition as a function of the coupling parameter for a fixed value of the temperature are plotted in Figure 4. For negative values of the coupling parameter (the region I in the figure), the first-order phase transition of CNTs takes place between a paranematic phase with a negative order parameter (perpendicular alignment) and a nematic phase with a positive order parameter (parallel alignment). For positive values of γ (region II in the figure), the transition takes place between a paranematic phase and a nematic phase, both with positive order parameters (parallel alignment). If the coupling increases the degrees of alignment of the two phases become smaller until the critical value of the coupling parameter when they are identical.

### 3.2 Phase diagram

The equilibrium phase diagram can be obtained by minimizing the free energy with respect to SCNT and SLC:

$$\frac{\partial \mathbf{f}}{\partial \mathbf{S}\_{\rm CNT}} = \frac{\partial \mathbf{f}}{\partial \mathbf{S}\_{\rm LC}} = \mathbf{0} \tag{7}$$

smaller case letters i, p, and n stand for isotropic, paranematic (parallel align-

Binary Mixture Composed of Nematic Liquid Crystal and Carbon Nanotubes: A Theoretical…

The Tð Þ ϕ phase diagram for a constant positive coupling parameter. The horizontal line shows the

For T < TNI, LC is in the nematic phase, and the paranematic-nematic phase transition of CNTs is first order. With decreasing temperature, the bi-phase region (the Flory "chimney" [45]) becomes smaller and cancels at the critical point (for the value <sup>γ</sup> <sup>¼</sup> <sup>40</sup>:33 N=m2, the critical temperature is given by Tc � TNI ¼ �7:84 K). On the contrary, for T > TNI, LC is in the isotropic phase. The isotropic-nematic phase transition of CNTs is first order with a constant Flory "chimney" that does not depend on temperature (because SLC ¼ 0, f LC ¼ f CNT=LC ¼ 0, and the problem is equivalent with the dispersion of CNTs in an isotropic solvent). The triple points are the intersection points between the CNT phase transition equilibrium curves and

To see in more detail the orientational order of the two components, in Figure 6, we have plotted the order parameter profiles SLC and SCNT along the binodal lines

The transition between the isotropic and nematic phases of LC is first order (see Figure 6a), and the values of the LC order parameter depend only on temperature and are not influenced by CNT phase transition (because of vCNT ≫ vLC, the concentration of LC component is much larger than for CNTs). But each particle contributes with kBT to the free energy, so that the free energy of LC is significantly larger than that of CNTs. The order parameters of CNTs as functions of temperature are shown in Figure 6b. Lowering the temperature, the jump of the order parameters cancels at the critical temperature. In the isotropic phase of LC

(T > TNI), the jump of the CNT order parameter remains constant independent on

The negative coupling parameter corresponds to a paranematic (SCNT,par very small and negative) and nematic (SCNT,nem large and positive) phase transition of CNTs. The corresponding Tð Þ ϕ phase diagram is shown in Figure 7, where the smaller case letters i, p, and n stand for isotropic, paranematic (perpendicular

For T < TNI, LC is in the nematic phase, and the paranematic (perpendicular) nematic (parallel) phase transition of CNTs is first order. Contrary to the positive coupling parameter, here with decreasing temperature, the bi-phase region (the Flory "chimney" [45]) becomes larger. For T > TNI, the characteristic of the phase

temperature (see the discussion of the results plotted in Figure 5).

ment), and nematic phases, respectively.

DOI: http://dx.doi.org/10.5772/intechopen.81936

isotropic-nematic phase transition of LC.

Figure 5.

as a function of temperature.

3.2.2 Negative coupling constant

39

alignment), and nematic phases, respectively.

LC phase transition equilibrium curve (the horizontal lines).

and equating the chemical potentials of CNTs and LC in the two phases. The chemical potentials are given by

$$\begin{aligned} \mu\_{\rm CNT} &= \nu\_{\rm CNT} \left[ f + (\mathbf{1} - \phi) \frac{\partial f}{\partial \phi} \right] \\ \mu\_{\rm LC} &= \nu\_{\rm LC} \left( f - \phi \frac{\partial f}{\partial \phi} \right) \end{aligned} \tag{8}$$

where the free energy density is given by Eq. (5).

### 3.2.1 Positive coupling constant

A positive coupling parameter corresponds to a paranematic (SCNT,par very small and positive) and nematic (SCNT,nem large and positive) phase transition of CNTs. The corresponding Tð Þ ϕ phase diagram is shown in Figure 5, where the

Binary Mixture Composed of Nematic Liquid Crystal and Carbon Nanotubes: A Theoretical… DOI: http://dx.doi.org/10.5772/intechopen.81936

Figure 5.

gap of CNTs remains practically constant, while for positive values (region II in the figure, parallel alignment), the volume fraction gap decreases with increasing γ

The order parameter of the two phases of CNTs at the transition as a function of the coupling parameter for a

Liquid Crystals - Self-Organized Soft Functional Materials for Advanced Applications

The equilibrium phase diagram can be obtained by minimizing the free energy

<sup>¼</sup> <sup>∂</sup><sup>f</sup> ∂SLC

and equating the chemical potentials of CNTs and LC in the two phases. The

<sup>μ</sup>CNT <sup>¼</sup> vCNT <sup>f</sup> <sup>þ</sup> ð Þ <sup>1</sup> � <sup>ϕ</sup> <sup>∂</sup><sup>f</sup>

A positive coupling parameter corresponds to a paranematic (SCNT,par very small and positive) and nematic (SCNT,nem large and positive) phase transition of CNTs. The corresponding Tð Þ ϕ phase diagram is shown in Figure 5, where the

<sup>μ</sup>LC <sup>¼</sup> vLC <sup>f</sup> � <sup>ϕ</sup> <sup>∂</sup><sup>f</sup>

where the free energy density is given by Eq. (5).

∂ϕ

(8)

∂ϕ

¼ 0 (7)

∂f ∂SCNT

The CNT order parameters at the transition as a function of the coupling parameter for a fixed value of the temperature are plotted in Figure 4. For negative values of the coupling parameter (the region I in the figure), the first-order phase transition of CNTs takes place between a paranematic phase with a negative order parameter (perpendicular alignment) and a nematic phase with a positive order parameter (parallel alignment). For positive values of γ (region II in the figure), the transition takes place between a paranematic phase and a nematic phase, both with positive order parameters (parallel alignment). If the coupling increases the degrees of alignment of the two phases become smaller until the critical value of the cou-

until it cancels for critical value γc.

fixed value of the temperature in the nematic region of LC.

pling parameter when they are identical.

3.2 Phase diagram

Figure 4.

with respect to SCNT and SLC:

chemical potentials are given by

3.2.1 Positive coupling constant

38

The Tð Þ ϕ phase diagram for a constant positive coupling parameter. The horizontal line shows the isotropic-nematic phase transition of LC.

smaller case letters i, p, and n stand for isotropic, paranematic (parallel alignment), and nematic phases, respectively.

For T < TNI, LC is in the nematic phase, and the paranematic-nematic phase transition of CNTs is first order. With decreasing temperature, the bi-phase region (the Flory "chimney" [45]) becomes smaller and cancels at the critical point (for the value <sup>γ</sup> <sup>¼</sup> <sup>40</sup>:33 N=m2, the critical temperature is given by Tc � TNI ¼ �7:84 K). On the contrary, for T > TNI, LC is in the isotropic phase. The isotropic-nematic phase transition of CNTs is first order with a constant Flory "chimney" that does not depend on temperature (because SLC ¼ 0, f LC ¼ f CNT=LC ¼ 0, and the problem is equivalent with the dispersion of CNTs in an isotropic solvent). The triple points are the intersection points between the CNT phase transition equilibrium curves and LC phase transition equilibrium curve (the horizontal lines).

To see in more detail the orientational order of the two components, in Figure 6, we have plotted the order parameter profiles SLC and SCNT along the binodal lines as a function of temperature.

The transition between the isotropic and nematic phases of LC is first order (see Figure 6a), and the values of the LC order parameter depend only on temperature and are not influenced by CNT phase transition (because of vCNT ≫ vLC, the concentration of LC component is much larger than for CNTs). But each particle contributes with kBT to the free energy, so that the free energy of LC is significantly larger than that of CNTs. The order parameters of CNTs as functions of temperature are shown in Figure 6b. Lowering the temperature, the jump of the order parameters cancels at the critical temperature. In the isotropic phase of LC (T > TNI), the jump of the CNT order parameter remains constant independent on temperature (see the discussion of the results plotted in Figure 5).

### 3.2.2 Negative coupling constant

The negative coupling parameter corresponds to a paranematic (SCNT,par very small and negative) and nematic (SCNT,nem large and positive) phase transition of CNTs. The corresponding Tð Þ ϕ phase diagram is shown in Figure 7, where the smaller case letters i, p, and n stand for isotropic, paranematic (perpendicular alignment), and nematic phases, respectively.

For T < TNI, LC is in the nematic phase, and the paranematic (perpendicular) nematic (parallel) phase transition of CNTs is first order. Contrary to the positive coupling parameter, here with decreasing temperature, the bi-phase region (the Flory "chimney" [45]) becomes larger. For T > TNI, the characteristic of the phase

Figure 6.

The order parameters along the binodal lines for a constant positive coupling parameter. (a) The LC order parameter and (b) the CNT order parameters.

4. Conclusions

parameter and (b) the CNT order parameters.

DOI: http://dx.doi.org/10.5772/intechopen.81936

Figure 8.

becomes continuous.

coupling strength γ.

41

In the present chapter, we have extended the previous mesoscopic phenomenological model [31, 32, 34–36] (used to describe the phase behavior of a binary mixture composed of CNTs and thermotropic nematic LC) to include the possibility of a perpendicular alignment of CNTs to LC molecules. The model contains the CNT free energy density (2), the Landau-de Gennes free energy (3) for thermotropic LC order, and an interaction term between the nematic CNTs and nematic LC (4). This interaction term generates the possibility of existence of two nematic phases of CNTs: (i) the mean direction of orientation of CNTs is parallel with the direction of the director of LC molecules, when SCNT > 0 and SLC > 0, and (ii) the two direction of orientation are perpendicular with each other, SCNT < 0 and SLC > 0. It is to be mentioned that the order parameter of CNTs can be negative (perpendicular alignment) only for a paranematic phase for which the degree of orientational order is very low. The model predicts in this case a first-order paranematic (perpendicular alignment)-nematic (parallel alignment) phase transition of CNTs. When the coupling constant is positive, the first-order paranematic (parallel alignment)-nematic (parallel alignment) phase transition of CNTs cancels at a critical point, when the transition

The order parameters along the binodal lines for a constant negative coupling parameter. (a) The LC order

Binary Mixture Composed of Nematic Liquid Crystal and Carbon Nanotubes: A Theoretical…

The phase behavior and orientational properties of the mixture are discussed considering different values of temperature T, volume fraction of CNTs ϕ, and

The theoretical model we have presented describes quite well (comparing with experimental results) the phase properties of the CNTs into thermotropic

#### Figure 7.

The Tð Þ ϕ phase diagram for a constant negative coupling parameter. The horizontal line shows the isotropic-nematic phase transition of LC.

diagram remains the same; because LC is in the isotropic phase, the isotropicnematic phase transition of CNTs is first order with a constant Flory "chimney" that does not depend on temperature.

The order parameter profiles SLC and SCNT along the binodal lines as a function of temperature are plotted in Figure 8.

Again the transition between the isotropic and nematic phases of LC is first order (see Figure 8a), and the values of the LC order parameter depend only on temperature. The behavior of CNT orientational order with temperature is shown in Figure 8b. In the nematic phase of LC (T < TNI), the CNT jump of the order parameters at transition slowly decreases with increasing temperature, while in the isotropic phase of LC (T > TNI), the jump of the CNT order parameter remains constant independent on temperature.

Binary Mixture Composed of Nematic Liquid Crystal and Carbon Nanotubes: A Theoretical… DOI: http://dx.doi.org/10.5772/intechopen.81936

Figure 8.

The order parameters along the binodal lines for a constant negative coupling parameter. (a) The LC order parameter and (b) the CNT order parameters.

## 4. Conclusions

In the present chapter, we have extended the previous mesoscopic phenomenological model [31, 32, 34–36] (used to describe the phase behavior of a binary mixture composed of CNTs and thermotropic nematic LC) to include the possibility of a perpendicular alignment of CNTs to LC molecules. The model contains the CNT free energy density (2), the Landau-de Gennes free energy (3) for thermotropic LC order, and an interaction term between the nematic CNTs and nematic LC (4). This interaction term generates the possibility of existence of two nematic phases of CNTs: (i) the mean direction of orientation of CNTs is parallel with the direction of the director of LC molecules, when SCNT > 0 and SLC > 0, and (ii) the two direction of orientation are perpendicular with each other, SCNT < 0 and SLC > 0. It is to be mentioned that the order parameter of CNTs can be negative (perpendicular alignment) only for a paranematic phase for which the degree of orientational order is very low. The model predicts in this case a first-order paranematic (perpendicular alignment)-nematic (parallel alignment) phase transition of CNTs. When the coupling constant is positive, the first-order paranematic (parallel alignment)-nematic (parallel alignment) phase transition of CNTs cancels at a critical point, when the transition becomes continuous.

The phase behavior and orientational properties of the mixture are discussed considering different values of temperature T, volume fraction of CNTs ϕ, and coupling strength γ.

The theoretical model we have presented describes quite well (comparing with experimental results) the phase properties of the CNTs into thermotropic

diagram remains the same; because LC is in the isotropic phase, the isotropicnematic phase transition of CNTs is first order with a constant Flory "chimney" that

The order parameters along the binodal lines for a constant positive coupling parameter. (a) The LC order

Liquid Crystals - Self-Organized Soft Functional Materials for Advanced Applications

The Tð Þ ϕ phase diagram for a constant negative coupling parameter. The horizontal line shows the

The order parameter profiles SLC and SCNT along the binodal lines as a function

Again the transition between the isotropic and nematic phases of LC is first order (see Figure 8a), and the values of the LC order parameter depend only on temperature. The behavior of CNT orientational order with temperature is shown in Figure 8b. In the nematic phase of LC (T < TNI), the CNT jump of the order parameters at transition slowly decreases with increasing temperature, while in the isotropic phase of LC (T > TNI), the jump of the CNT order parameter remains

does not depend on temperature.

isotropic-nematic phase transition of LC.

parameter and (b) the CNT order parameters.

Figure 7.

40

Figure 6.

of temperature are plotted in Figure 8.

constant independent on temperature.

nematic LC. The model could be improved by considering the polydispersity of the CNT component and by considering, in more detail, the form of the interaction energy between the two components.

References

16:865-869

Today. 2007;16:1

[1] Lynch MD, Patrick DL. Organizing carbon nanotubes with liquid crystals.

DOI: http://dx.doi.org/10.5772/intechopen.81936

[11] Ji Y, Huang YY, Terentjev EM. Dissolving and alignment carbon nanotubes in thermotropic liquid crystals. Langmuir. 2011;27:13254

Binary Mixture Composed of Nematic Liquid Crystal and Carbon Nanotubes: A Theoretical…

[12] Lebovka NI, Lisetski LN, Goncharuk AI, Minenko SS, Ponevchinsky VV, Soskin MS. Phase transitions in

smectogenic liquid crystal BBBA doped by multiwall carbon nanotubes. Phase

[13] Kumar S. Nanoparticles in the supramolecular order of discotic liquid crystals. Liquid Crystals. 2014;41:353

[14] Weiss V, Thiruvengadathan R,

characterization of a carbon nanotubelyotropic liquid crystal composite. Langmuir. 2006;22:854-856

[15] Lagerwall J, Scalia G, Haluska M, Dettlaff-Weglikowska U, Roth S, Giesselmann F. Nanotubes alignment using lyotropic liquid crystal. Advanced

[16] Schymura S, Enz E, Roth S, Scalia G, Lagerwall JPF. Macroscopic-scale carbon nanotube alignment via selfassembly in lyotropic liquid crystals. Synthetic Metals. 2009;159:2177

[17] Ould-Moussa N, Blanc C, Zamora-

Smalyukh II, Islam MF, et al. Dispersion and orientation of single-walled carbon nanotubes in a chromonic liquid crystal.

[18] Duran H, Gazdecki B, Yamashita A, Kyu T. Effect of carbon nanotubes on phase transition of nematic liquid crystals. Liquid Crystals. 2005;32:815

[19] Chen HY, Lee W, Clark NA. Faster electro-optical response characteristic of a carbon-nanotube-nematic suspension.

Ledezma C, Lavrentovich OD,

Liquid Crystals. 2013;40:1628

Transitions. 2013;86:463

Regev O. Preparation and

Materials. 2007;19:359

[2] Dierking I, Scalia G, Morales P, LeClere D, Adv D. Aligning and reoriented carbon nanotubes with nematic liquid crystals. Maternité. 2004;

[3] Dierking I, San SE. Magnetically steered liquid crystal-nanotube switch. Applied Physics Letters. 2005;87:233507

[4] Zakri C. Carbon nanotubes and liquid crystalline phases. Liquid Crystal

[5] Lagerwall JPF, Scalia G. Carbon nanotubes in liquid crystals. Journal of Materials Chemistry. 2008;18:2890

Physics. 2009;42:063001

2010;11:333

43

[7] Scalia G. Alignment of carbon nanotubes in thermotropic and lyotropic

liquid crystals. ChemPhysChem.

[8] Lagerwall JPF, Scalia G. A new era for liquid crystal research: Application of liquid crystals in soft matter nano-, bio-, and microtehnology. Current Applied Physics. 2012;12:1387

[9] Dierking I, Scalia G, Morales P. Liquid crystal- carbon nanotubes dispersions. Journal of Applied Physiology. 2005;97:044309

[10] Schymura S, Kuhnast M, Lutz V, Jagiella S, Dettiaff-Weglikowska U, Roth S, et al. Towards efficient dispersion of carbon nanotubes in thermotropic liquid crystals. Advanced Functional Materials. 2010;20:3350

[6] Rahman M, Lee W. Scientific duo of carbon nanotubes and nematic liquid crystals. Journal of Physics D: Applied

Nano Letters. 2002;2:1197

## Author details

Vlad Popa-Nita<sup>1</sup> \* and Robert Repnik<sup>2</sup>

1 Faculty of Physics, University of Bucharest, Bucharest, Romania

2 Faculty of Natural Sciences and Mathematics, University of Maribor, Maribor, Slovenia

\*Address all correspondence to: v.popanita@gmail.com

© 2018 The Author(s). Licensee IntechOpen. This chapter is distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/ by/3.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Binary Mixture Composed of Nematic Liquid Crystal and Carbon Nanotubes: A Theoretical… DOI: http://dx.doi.org/10.5772/intechopen.81936

## References

nematic LC. The model could be improved by considering the polydispersity of the CNT component and by considering, in more detail, the form of the inter-

Liquid Crystals - Self-Organized Soft Functional Materials for Advanced Applications

action energy between the two components.

Author details

Vlad Popa-Nita<sup>1</sup>

Slovenia

42

\* and Robert Repnik<sup>2</sup>

\*Address all correspondence to: v.popanita@gmail.com

provided the original work is properly cited.

1 Faculty of Physics, University of Bucharest, Bucharest, Romania

2 Faculty of Natural Sciences and Mathematics, University of Maribor, Maribor,

© 2018 The Author(s). Licensee IntechOpen. This chapter is distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/ by/3.0), which permits unrestricted use, distribution, and reproduction in any medium, [1] Lynch MD, Patrick DL. Organizing carbon nanotubes with liquid crystals. Nano Letters. 2002;2:1197

[2] Dierking I, Scalia G, Morales P, LeClere D, Adv D. Aligning and reoriented carbon nanotubes with nematic liquid crystals. Maternité. 2004; 16:865-869

[3] Dierking I, San SE. Magnetically steered liquid crystal-nanotube switch. Applied Physics Letters. 2005;87:233507

[4] Zakri C. Carbon nanotubes and liquid crystalline phases. Liquid Crystal Today. 2007;16:1

[5] Lagerwall JPF, Scalia G. Carbon nanotubes in liquid crystals. Journal of Materials Chemistry. 2008;18:2890

[6] Rahman M, Lee W. Scientific duo of carbon nanotubes and nematic liquid crystals. Journal of Physics D: Applied Physics. 2009;42:063001

[7] Scalia G. Alignment of carbon nanotubes in thermotropic and lyotropic liquid crystals. ChemPhysChem. 2010;11:333

[8] Lagerwall JPF, Scalia G. A new era for liquid crystal research: Application of liquid crystals in soft matter nano-, bio-, and microtehnology. Current Applied Physics. 2012;12:1387

[9] Dierking I, Scalia G, Morales P. Liquid crystal- carbon nanotubes dispersions. Journal of Applied Physiology. 2005;97:044309

[10] Schymura S, Kuhnast M, Lutz V, Jagiella S, Dettiaff-Weglikowska U, Roth S, et al. Towards efficient dispersion of carbon nanotubes in thermotropic liquid crystals. Advanced Functional Materials. 2010;20:3350

[11] Ji Y, Huang YY, Terentjev EM. Dissolving and alignment carbon nanotubes in thermotropic liquid crystals. Langmuir. 2011;27:13254

[12] Lebovka NI, Lisetski LN, Goncharuk AI, Minenko SS, Ponevchinsky VV, Soskin MS. Phase transitions in smectogenic liquid crystal BBBA doped by multiwall carbon nanotubes. Phase Transitions. 2013;86:463

[13] Kumar S. Nanoparticles in the supramolecular order of discotic liquid crystals. Liquid Crystals. 2014;41:353

[14] Weiss V, Thiruvengadathan R, Regev O. Preparation and characterization of a carbon nanotubelyotropic liquid crystal composite. Langmuir. 2006;22:854-856

[15] Lagerwall J, Scalia G, Haluska M, Dettlaff-Weglikowska U, Roth S, Giesselmann F. Nanotubes alignment using lyotropic liquid crystal. Advanced Materials. 2007;19:359

[16] Schymura S, Enz E, Roth S, Scalia G, Lagerwall JPF. Macroscopic-scale carbon nanotube alignment via selfassembly in lyotropic liquid crystals. Synthetic Metals. 2009;159:2177

[17] Ould-Moussa N, Blanc C, Zamora-Ledezma C, Lavrentovich OD, Smalyukh II, Islam MF, et al. Dispersion and orientation of single-walled carbon nanotubes in a chromonic liquid crystal. Liquid Crystals. 2013;40:1628

[18] Duran H, Gazdecki B, Yamashita A, Kyu T. Effect of carbon nanotubes on phase transition of nematic liquid crystals. Liquid Crystals. 2005;32:815

[19] Chen HY, Lee W, Clark NA. Faster electro-optical response characteristic of a carbon-nanotube-nematic suspension.

Applied Physics Letters. 2007;90: 033510

[20] Basu R, Iannacchione GS. Carbon nanotube dispersed liquid crystal: A nano electromechanical system. Applied Physics Letters. 2009;95:173113

[21] Basu R, Iannacchione GS. Orientational coupling enhancement in a carbon nanotube dispersed liquid crystal. Physical Review E. 2010;81: 051705

[22] Sigdel KP, Iannacchione GS. Effect of carbon nanotubes on the isotropic to nematic and the nematic to smectic-A phase transitions in liquid crystal and carbon nanotubes composites. European Physical Journal E: Soft Matter and Biological Physics. 2011;34:34

[23] Schymura S, Scalia G. On the effect of carbon nanotubes on properties of liquid crystals. Philosophical Transactions of the Royal Society A. 2013;371:20120261

[24] Lee KJ, Park HG, Jeong HC, Kim DH, Seo DS, Lee JW, et al. Enhanced electro-optical behavior of a liquid crystal system via multi-walled carbon nanotube doping. Liquid Crystals. 2014; 41:25

[25] Basu R, Iannacchione GS. Dielectric hysteresis, relaxation dynamics, and nonvolatile memory effect in carbon nanotube dispersed liquid crystal. Journal of Applied Physics. 2009;106: 124312

[26] Somoza AM, Sagui C, Roland C. Liquid crystal phases of capped carbon nanotubes. Physical Review B. 2001;63: 081403-1

[27] Sabba Y, Thomas EL. Highconcentration dispersion of single-wall carbon nanotube. Macromolecules. 2004;37:4815

[28] Green MJ, Parra-Vasquez ANG, Behabtu N, Pasquali M. Modelling the phase behavior of polydispersed rigid rods with attractive interaction with application to single-walled carbon nanotubes in superacids. The Journal of Chemical Physics. 2009;131:084901

[37] Green MJ, Behabtu N, Pasquali M, Adams WW. Nanotubes as polymers.

DOI: http://dx.doi.org/10.5772/intechopen.81936

[47] Song W, Kinloch IA, Windle AH. Nematic liquid crystallinity of multiwall carbon nanotubes. Science. 2003;302:

[48] Song W, Windle AH. Isotropicnematic phase transition of dispersion of multiwall carbon nanotubes. Macromolecules. 2005;38:6181

[49] Faetti S, Palleschi V. Measurements of the interfacial tension between nematic and isotropic phase of some cyanobiphenyls. The Journal of Chemical Physics. 1984;81:6254

[50] Faetti S, Palleschi V. Nematicisotropic interface of some members of the homologous series of 4-cyano-4'-(nalkyl)biphenyl liquid crystals. Physical

[51] Faetti S, Palleschi V. Molecular orientation and anchoring energy at the nematic-isotropic. Journal de Physique

Lettres (France). 1984;45:L313

Review A. 1984;30:3241

1363

Binary Mixture Composed of Nematic Liquid Crystal and Carbon Nanotubes: A Theoretical…

[38] Onsager L. The effect of shape on the interaction of colloidal particles. Annals of the New York Academy of

[39] de Gennes PG, Prost J. The Physics of Liquid Crystals. Oxford: Oxford

[40] Oswald P, Pieranski P. Nematic and cholesteric liquid crystals; concepts and physical properties illustrated by experiments. In: Liquid Crystals Book Series. Boca Raton: Taylor and Francis

[41] Doi M. Molecular dynamics and rheological properties of concentrated solutions of rodlike polymer in isotropic and liquid crystalline phases. Journal of Polymer Science Part B: Polymer

[42] Doi M, Edwards SF. Theory of Polymer Dynamics. Oxford: Clarendon;

[43] Kuzuu N, Doi M. Constitutive equations for nematic liquid crystals under weak velocity gradient derived from a molecular kinetic equation. Journal of the Physical Society of Japan.

[44] Park KA, Lee SM, Lee SH, Lee YH. Anchoring a liquid crystal molecule on a single-walled carbon nanotube. Journal of Physical Chemistry C. 2007;111:1620

[45] Flory PJ. Principles of Polymer Chemistry. Ithaca: Cornell University

of semi-flexible chain molecules. Proceedings of the Royal Society of

London A. 1956;243:73

[46] Flory PJ. Statistical thermodynamics

Polymer. 2009;50:4979

Sciences. 1949;51:727

University Press; 1993

Group/CRC Press; 2005

Physics. 1981;19:229

1989

1983;52:3486

Press; 1953

45

[29] Matsuyama A, Kato T. Phase separation in mixture of a liquid crystal and a nanocolloidal particle. Physics Review. 1999;E59:763

[30] Matsuyama A. Theory of binary mixture of a rodlike polymer and a liquid crystal. The Journal of Chemical Physics. 2010;132:214902

[31] van der Schoot P, Popa-Nita V, Kralj S. Alignment of carbon nanotubes in nematic liquid crystals. The Journal of Physical Chemistry. B. 2008;112:4512

[32] Popa-Nita V, Kralj S. Liquid crystalcarbon nanotubes mixtures. The Journal of Chemical Physics. 2010;132:024902

[33] Lisetski LN, Lebovka NI, Naydenov SV, Soskin MS. Dispersions of multiwalled carbon nanotubes in liquid crystals: A physical picture of aggregation. Journal of Molecular Liquids. 2011;164:143

[34] Popa-Nita V, Barna V, Repnick R, Kralj S. In: Suzuki S, editor. Syntheses and Applications of Carbon Nanotubes and Their Composites. Rijeka, Croatia: InTech; 2013. Chap. 7

[35] Popa-Nita V. Mixtures composed of liquid crystals and carbon nanotubes. The Journal of Chemical Physics. 2014; 140:164905

[36] Popa-Nita V. The phase behavior of rigid rods in an anisotropic mean field with application to carbon nanotubes in nematic liquid crystals. The Journal of Chemical Physics. 2015;143:094901

Binary Mixture Composed of Nematic Liquid Crystal and Carbon Nanotubes: A Theoretical… DOI: http://dx.doi.org/10.5772/intechopen.81936

[37] Green MJ, Behabtu N, Pasquali M, Adams WW. Nanotubes as polymers. Polymer. 2009;50:4979

Applied Physics Letters. 2007;90:

Physics Letters. 2009;95:173113

[21] Basu R, Iannacchione GS.

[20] Basu R, Iannacchione GS. Carbon nanotube dispersed liquid crystal: A nano electromechanical system. Applied

Liquid Crystals - Self-Organized Soft Functional Materials for Advanced Applications

[28] Green MJ, Parra-Vasquez ANG, Behabtu N, Pasquali M. Modelling the phase behavior of polydispersed rigid rods with attractive interaction with application to single-walled carbon nanotubes in superacids. The Journal of Chemical Physics. 2009;131:084901

[29] Matsuyama A, Kato T. Phase separation in mixture of a liquid crystal and a nanocolloidal particle. Physics

[30] Matsuyama A. Theory of binary mixture of a rodlike polymer and a liquid crystal. The Journal of Chemical

[31] van der Schoot P, Popa-Nita V, Kralj S. Alignment of carbon nanotubes in nematic liquid crystals. The Journal of Physical Chemistry. B. 2008;112:4512

[32] Popa-Nita V, Kralj S. Liquid crystalcarbon nanotubes mixtures. The Journal of Chemical Physics. 2010;132:024902

[33] Lisetski LN, Lebovka NI, Naydenov SV, Soskin MS. Dispersions of multiwalled carbon nanotubes in liquid crystals: A physical picture of aggregation. Journal of Molecular

[34] Popa-Nita V, Barna V, Repnick R, Kralj S. In: Suzuki S, editor. Syntheses and Applications of Carbon Nanotubes and Their Composites. Rijeka, Croatia:

[35] Popa-Nita V. Mixtures composed of liquid crystals and carbon nanotubes. The Journal of Chemical Physics. 2014;

[36] Popa-Nita V. The phase behavior of rigid rods in an anisotropic mean field with application to carbon nanotubes in nematic liquid crystals. The Journal of Chemical Physics. 2015;143:094901

Review. 1999;E59:763

Physics. 2010;132:214902

Liquids. 2011;164:143

InTech; 2013. Chap. 7

140:164905

Orientational coupling enhancement in a carbon nanotube dispersed liquid crystal. Physical Review E. 2010;81:

[22] Sigdel KP, Iannacchione GS. Effect of carbon nanotubes on the isotropic to nematic and the nematic to smectic-A phase transitions in liquid crystal and carbon nanotubes composites. European Physical Journal E: Soft Matter and Biological Physics. 2011;34:34

[23] Schymura S, Scalia G. On the effect of carbon nanotubes on properties of

Transactions of the Royal Society A.

[24] Lee KJ, Park HG, Jeong HC, Kim DH, Seo DS, Lee JW, et al. Enhanced electro-optical behavior of a liquid crystal system via multi-walled carbon nanotube doping. Liquid Crystals. 2014;

[25] Basu R, Iannacchione GS. Dielectric hysteresis, relaxation dynamics, and nonvolatile memory effect in carbon nanotube dispersed liquid crystal. Journal of Applied Physics. 2009;106:

[26] Somoza AM, Sagui C, Roland C. Liquid crystal phases of capped carbon nanotubes. Physical Review B. 2001;63:

[27] Sabba Y, Thomas EL. Highconcentration dispersion of single-wall carbon nanotube. Macromolecules.

liquid crystals. Philosophical

2013;371:20120261

41:25

124312

081403-1

2004;37:4815

44

033510

051705

[38] Onsager L. The effect of shape on the interaction of colloidal particles. Annals of the New York Academy of Sciences. 1949;51:727

[39] de Gennes PG, Prost J. The Physics of Liquid Crystals. Oxford: Oxford University Press; 1993

[40] Oswald P, Pieranski P. Nematic and cholesteric liquid crystals; concepts and physical properties illustrated by experiments. In: Liquid Crystals Book Series. Boca Raton: Taylor and Francis Group/CRC Press; 2005

[41] Doi M. Molecular dynamics and rheological properties of concentrated solutions of rodlike polymer in isotropic and liquid crystalline phases. Journal of Polymer Science Part B: Polymer Physics. 1981;19:229

[42] Doi M, Edwards SF. Theory of Polymer Dynamics. Oxford: Clarendon; 1989

[43] Kuzuu N, Doi M. Constitutive equations for nematic liquid crystals under weak velocity gradient derived from a molecular kinetic equation. Journal of the Physical Society of Japan. 1983;52:3486

[44] Park KA, Lee SM, Lee SH, Lee YH. Anchoring a liquid crystal molecule on a single-walled carbon nanotube. Journal of Physical Chemistry C. 2007;111:1620

[45] Flory PJ. Principles of Polymer Chemistry. Ithaca: Cornell University Press; 1953

[46] Flory PJ. Statistical thermodynamics of semi-flexible chain molecules. Proceedings of the Royal Society of London A. 1956;243:73

[47] Song W, Kinloch IA, Windle AH. Nematic liquid crystallinity of multiwall carbon nanotubes. Science. 2003;302: 1363

[48] Song W, Windle AH. Isotropicnematic phase transition of dispersion of multiwall carbon nanotubes. Macromolecules. 2005;38:6181

[49] Faetti S, Palleschi V. Measurements of the interfacial tension between nematic and isotropic phase of some cyanobiphenyls. The Journal of Chemical Physics. 1984;81:6254

[50] Faetti S, Palleschi V. Nematicisotropic interface of some members of the homologous series of 4-cyano-4'-(nalkyl)biphenyl liquid crystals. Physical Review A. 1984;30:3241

[51] Faetti S, Palleschi V. Molecular orientation and anchoring energy at the nematic-isotropic. Journal de Physique Lettres (France). 1984;45:L313

**47**

Section 3

Electro-Optic

Switching Behavior and

Photorefractive Effect

in Ferroelectric Liquid

Crystals

## Section 3
